synthesis of phosphorus-containing polyurethanes and poly ... ?· synthesis of...
Post on 08-May-2019
Embed Size (px)
Turk J Chem
(2017) 41: 630 647
Turkish Journal of Chemistry
http :// journa l s . tub i tak .gov . t r/chem/
Synthesis of phosphorus-containing polyurethanes and poly(urethane-acrylate)s
Mahir Burak SUDEMEN1,, Hacer Aysen ONEN21Department of Polymer Science and Technology, Institute of Sciences and Technology,
Istanbul Technical University, Istanbul, Turkey2Department of Chemistry, Faculty of Sciences and Letters, Istanbul Technical University, Istanbul, Turkey
Received: 14.10.2016 Accepted/Published Online: 03.02.2017 Final Version: 10.11.2017
Abstract: Solvent-based polyurethanes and poly(urethane-acrylate)s were synthesized using phosphorus-containing
polyester polyols in order to compare the thermal properties of different polymer types. Since the location of the
phosphorus group might have vital importance when comparing the thermal properties, phosphorus groups were kept
on the pendant chains in poly(urethane-acrylate)s using phosphorus-containing urethane macromonomers while they
were kept on the backbone in polyurethanes. The effect of molar mass of polyurethanes and pendant urethane chains of
poly(urethane-acrylate)s on thermal properties was also investigated. Characterization of the synthesized polymers was
carried out using FT-IR, GPC, NMR, and DSC followed by evaluation of the thermal properties.
Key words: Polyurethane, poly(urethane-acrylate), phosphorus flame retardant
Research on high performance coating polymers has long been an interest for both the academic and industrial
communities. In the last few decades, researchers have systematically created new approaches for coating
polymers to meet the requirements of the application areas. One of the coating polymers that has gained
importance in the last few decades in the industry is polyurethane. Polyurethane coatings find applications in
many industries such as textile, leather, paint, aerospace, and metal coating in an increasing trend due to their
advantageous properties such as mechanical durability, chemical resistance, and low temperature curing along
with their highly elastomeric properties.15 On the other hand, the main disadvantage of polyurethanes is their
high price in the market due to expensive raw materials such as di-isocyanates. In addition to the high cost,
the production of polyurethanes is more problematic compared to the other polymerization systems due to the
high reactivity of isocyanates with impurities such as water.6
Another important polymer type used in the coating industry is acrylic polymer. While the mechanical
properties and chemical resistances of acrylic polymers are inferior compared to polyurethanes, their cost
efficiency is making them the choice for low cost applications. The ability to tailor the required properties
using the wide selection of commercially available acrylic monomers also makes this polymer type useful for
coating industries such as paint, garment, furniture, and textile.
The disadvantages of both polyurethane and polyacrylate coatings are somewhat overcome by hybrid
coatings. One of the methods for obtaining optimized properties is through physical blending of the polyurethane
and polyacrylate.7 While higher mechanical properties, solvent and chemical resistances, and toughness are
SUDEMEN and ONEN/Turk J Chem
gained by polyurethanes, lower cost and outdoor resistance are provided by polyacrylates. Although it is a
simple and effective way to achieve some of the hybrid properties, physical blending fails to provide the desired
properties in performance coatings.8 Another method researchers focus on is emulsion acrylic polymerization
using polyurethane dispersions as the emulsifier.912 In this case, the resulting polymer network generates
more durable polymers compared to a simple blending system. However, this system fails to overcome the
shortcomings of blending technology. For this reason, research on covalently bonded hybrid systems is recently
attracting a lot of attention using urethane and acrylate chemistry. Covalent hybrid systems focus on the
polymerization of acrylic terminated urethane macromonomers with acrylic monomers.1318 One of the distinct
advantages of this method in performance coating development is the ability to combine different monomer types
of the two different polymer technologies in order to obtain the desired properties from the coated substrate.
In addition to the benefits gained by chemical versatility, the structural differences offered by urethane-
acrylate polymers might provide interesting properties compared to linear polyurethanes or polyacrylates.
Even though there are a variety of studies on the polymerization of urethane macromonomers with acrylic
monomers, there are no reports that compare the final properties of poly(urethane-acrylate)s with those of
linear polyurethanes. Therefore, in order to understand the effect of structural differences between linear
polyurethanes and poly(urethane-acrylate)s on the final properties of polymers, we designed and synthesized
phosphorus-containing polyurethanes and poly(urethane-acrylate)s. Phosphorus is kept on the backbone of
polyurethanes and on the pendant urethane macromonomers of poly(urethane-acrylate)s in order to compare the
efficiency of pendant chains of poly(urethane-acrylate)s with linear polyurethanes on thermal properties. After
the polymerizations, the effect of phosphorus content and molar mass on the thermal properties of poly(urethane-
acrylate)s and linear polyurethanes were discussed.
2. Results and discussion
2.1. Synthesis of polyester polyols
Polyester polyols (PEPs) with two different molar masses were synthesized using adipic acid, 1,6-hexanediol,
and neopentyl glycol via an esterification reaction as shown in Figure 1. The synthesized polyester polyols were
designated as PEP-L and PEP-H, with L and H indicating low and high molar masses, respectively.
Figure 1. Synthesis of polyester polyols.
FT-IR spectra of the polyester polyols showed major polyester bands at 1729 cm1 , 2866/2936 cm1 , and
1371 cm1 arising from carbonyl stretching vibration, CH2 symmetric and asymmetric stretching vibrations,
SUDEMEN and ONEN/Turk J Chem
and gem-dimethyl stretching vibration of neopentyl glycol, respectively, as shown in Figure 2. The free hydroxyl
group appeared as a broad band around 3500 cm1 .
Figure 2. FT-IR spectrum of polyester polyol.
Phosphorus-containing polyester polyols (PPEPs) with varying phosphorus contents were synthesized as
shown in Figure 3. In order to adjust the phosphorus contents, the molar ratio of phenyl dichlorophosphate
and PEP-L/PEP-H was changed. While two of the PPEPs, PPEP-LP and PPEP-HP, were synthesized using
PEP-H to be used in the synthesis of polyurethanes, the other two PPEPs, PPEP-LM and PPEP-HM, were
synthesized using PEP-L to be used in the synthesis of macromonomers.
Figure 3. Synthesis of phosphorus-containing polyester polyols.
SUDEMEN and ONEN/Turk J Chem
After the reaction of synthesized polyester polyols with phenyl dichlorophosphate in order to obtain
phosphorus-containing polyester polyols, new bands appeared in the FT-IR spectra as shown in Figure 4.
Bands at 1593 cm1 and 1491 cm1 were attributed to the stretching vibrations of the phenyl group on the
polyester polyol backbone. Bands at 1256 cm1 , 1015 cm1 , and 939 cm1 arose from P=O stretching, P
OC asymmetric stretching, and POPh symmetric stretching, respectively. The monosubstituted phenyl ring
showed a strong band at 767 cm1 .
Figure 4. FT-IR spectrum of phosphorus-containing polyester polyol.
DSC studies showed two different transitions for both Tg and Tm of polyester polyols. While Tg values
lower than 58 C appeared as the major transitions, values at higher temperatures showed minor transitions.
The two different Tg and Tm values could be due to distribution of the monomers throughout the polyols.
While polyol chains containing more 1,6-hexanediol in the backbone will create polyols with higher Tg and
Tm values, chains containing more neopentyl glycol will result in lower Tg and Tm values. After the reaction
of polyester polyols with phenyl dichlorophosphate, both Tg and Tm values increased as shown in Table 1.
Increases in the values in both transitions indicate successful incorporation of phenyl phosphate moiety.
Table 1. Thermal transitions of polyester polyols.
Polyester polyolsTg1 Tg2 Tm1 Tm2
PEP-H 69.7 C 30.8 C 14.1 C 26.1 CPEP-L 71.6 C 32.4 C 16.8 C 25.4 CPPEP-LP 67.0 C 26.1 C 31.2 C 39.8 CPPEP-HP 65.2 C 22.8 C 32.6 C 41.4 CPPEP-LM 64.8 C 23.4 C 35.1 C 41.6 CPPEP-HM 58.1 C 18.3 C 35.3 C 43.8 C
SUDEMEN and ONEN/Turk J Chem
2.2. Synthesis of polyurethanes
Synthesized phosphorus-containing polyester polyols were subsequently used in the synthesis of the phosphorus-
containing polyurethanes with low and high phosphorus contents (LPC HPC), which were 0.63%0.64% and
1.11%1.12% over dry mass. Polyurethanes were synthesized in two different molar masses for each phosphorus
content in order to see the effect of molar mass on char yields. Molar masses